Broadband Photoresponse Enhancement of a High‐Performance...
Embed Size (px)
Transcript of Broadband Photoresponse Enhancement of a High‐Performance...
FU LL P
A P ER
© 2016 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim 6641wileyonlinelibrary.com
photodetectors response to wide range of light and satisfy the requirements of broadband light communication, imaging sensing, etc. [ 10,11 ] In particular, UV–visible photodetectors are one type of important broadband photodetectors that detect light from UV to visible range through the use of a single detector. To realize UV–vis- ible light detection, materials with pho- toresponse in this broadband region are necessary. Silicon is the most widely used material among semiconductor materials as broadband photodetectors via metal– oxide–semiconductor (MOS) structure for its compatibility with current semicon- ductor industry. Nevertheless, a very thin oxide layer can cause large leakage current and a premature voltage broken down. [ 12 ] Hence, some other materials for UV–vis-
ible light detection are explored such as MoS 2 , CdSe, In 2 Se 3 , and organic perovskites. [ 13–16 ] However, photodetectors based on these materials usually suffer seriously from instability, which impedes their wider application. Therefore, new strate- gies for high-performance broadband UV–visible light detec- tion are necessary.
As a promising candidate for fabricating a high-performance broadband photodetector, p-type semiconductor Se exhibits many excellent properties. [ 17 ] For example, the band gap of Se is about 1.67 eV, [ 18 ] which means that Se exhibits broadband photoresponse from visible to UV region. Previous works also demonstrate that the conductivity of Se can rise from 10 −6 to 10 −5 Ω −1 cm −1 to 0.59 Ω −1 cm −1 under ≈10 −4 µW µm −2 633 nm laser illumination. [ 19,20 ] Furthermore, the response time of ele- mental selenium is very fast. The response time of amorphous Se fi lm or Se nanobelts metal–semiconductor–metal (MSM) photodetector reaches several milliseconds, [ 18,21 ] much higher than ZnO, ZnS, and MoS 2 with a similar MSM structure. [ 13,22,23 ] Se microstructures synthesized by vapor phase deposition attract many interests for low cost, good crystallization, easy to build device, fast response, and also broadband photoresponse. In spite of these advantages, the responsivity of Se microstruc- ture photodetectors is still lower than expected.
Recently, with the unique ability to route and manipulate light at nanoscale beyond the diffraction limit, surface plasmon resonance arising from metallic nanoparticles (NPs) offers new opportunities to improve the performance of optoelectronic devices. [ 24,25 ] Up to now, it has demonstrated signifi cant potential
Broadband Photoresponse Enhancement of a High- Performance t -Se Microtube Photodetector by Plasmonic Metallic Nanoparticles
Kai Hu , Hongyu Chen , Mingming Jiang , Feng Teng , Lingxia Zheng , and Xiaosheng Fang *
Broadband responsivity enhancement of single Se microtube (Se-MT) photodetectors in the UV–visible region is presented in this research. The pristine Se-MT photodetector demonstrates broadband photoresponse from 300 to 700 nm with peak responsivity of ≈19 mA W −1 at 610 nm and fast speed (rise time 0.32 ms and fall time 23.02 ms). To further enhance the responsivity of the single Se-MT photodetector, Au and Pt nanoparticles (NPs) are sputtered on these devices. In contrast to only enhancement of responsivity in UV region by Pt NPs, broadband responsivity enhancement (≈600% to ≈800%) of the Se-MT photodetector is realized from 300 to 700 nm by tuning the size and density of Au NPs. The broadband responsivity enhancement phenomena are interpreted by both the surface modifi cation and surface plasmon coupling. The experimental results of this work provide an additional opportunity for fabricating high-performance UV–visible broadband photodetectors.
K. Hu, Dr. H. Y. Chen, Dr. F. Teng, Dr. L. X. Zheng, Prof. X. S. Fang Department of Materials Science Fudan University Shanghai 200433 , P. R. China E-mail: firstname.lastname@example.org Dr. M. M. Jiang State Key Laboratory of Luminescence and Applications Changchun Institute of Optics Fine Mechanics and Physics Chinese Academy of Sciences Changchun 130033 , P. R. China
Photodetectors with the ability to convert light (UV, visible, or infrared) into electric signal are fundamental to human life and have various applications including environmental monitoring, video-recording, ozone sensing, and optical communication. [ 1–5 ] In terms of the operation wavelength range, they are generally categorized into two types: special wavelength photodetectors and broadband photodetectors. [ 6 ] Special wavelength photode- tectors response to certain narrow range of wavelength, [ 7 ] such as a solar-blind photodetector that operates from 220 to 280 nm [ 8 ] and an even photodetector with an enhanced UV photoresponse in a narrow spectrum range of only 17 nm. [ 9 ] In contrast to special wavelength photodetectors, broadband
Adv. Funct. Mater. 2016, 26, 6641–6648
P A P ER
6642 wileyonlinelibrary.com © 2016 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim
for improving the performance of light- emitting diodes, lasers, solar cells, and espe- cially responsivity of photodetectors. [ 26,27 ] The additional tremendous local electro- magnetic fi elds are attributed to the redis- tributing surface charges of metallic NPs. And their surface charges can be modifi ed by changing shapes, distances, and materials of metallic NPs. This allows one to tailor the surface plasmon resonance frequency and manipulate scattering from the NPs over a broad wavelength range. [ 28,29 ] Even so, recent researches mainly focus on the selec- tive enhancement photodetection of surface plasmon in a narrow wavelength range. [ 30,31 ] Concerning the UV to visible photoresponse of Se semiconductor, broadband enhance- ment in UV–visible region is needed.
In this paper, Se microtubes (Se-MTs) are successfully prepared via a facile vapor transport and deposition route. After that, a single Se-MT is constructed into photo- detector device using indium as electrodes. Broadband (300–700 nm) and fast (rise time of 0.32 ms and fall time of 23.02 ms) pho- toresponses are realized by the Se-MT with peak responsivity of ≈19 mA W −1 at 610 nm. The photoresponse enhancement effect of Pt and Au NPs on single Se-MT photode- tectors is studied and it demonstrates that broadband enhancement of responsivity has been realized by Au nanoparticles, while only UV range (300–400 nm) enhancement has been found by Pt NPs. The results show that by coupling plasmonic Au NPs on surface of Se-MT photodetectors, ≈600% to ≈800% improvement of responsivity is realized in wideband range (≈300 to ≈700 nm). To get insight into the enhancement mechanism, theoretical analysis in conjunction with fi nite dif- ference time-domain (FDTD) method is also performed in the following. The method of fabricating single Se-MT-based pho- todetector and its broadband responsivity enhancement by Au NPs is expected to apply to UV–visible light detection.
2. Results and Discussion
Figure 1 shows the fi eld-emission scanning electron micros- copy (FESEM) characterization of as prepared Se-MTs with a large scale. The width of Se tubes varies from several microm- eters to tens of micrometers and the length of Se-MTs can reach several millimeters as depicted in Figure 1 a. The mag- nifi ed image in Figure 1 b reveals that Se-MTs are in hexagon shape with a hollow tubular morphology. Figure 1 c,d shows a typical single Se-MT with a length of 760 µm, a uniform width of 24 µm along the whole single microtube and one edge length of the tube of 8.8 µm. The phases of as prepared tubes are further confi rmed by X-ray diffraction (XRD) patterns as shown in Figure 2 a. The sharp diffraction peaks demon- strate good crystallinity of Se-MTs. All diffraction peaks can be
assigned to trigonal selenium ( t -Se, JCPDS No. 65-1876) with the lattice parameters of a = b = 4.364 Å, c = 4.959 Å. Figure 2 b presents the UV–visible absorption and refl ection spectra within 350–700 nm range of as prepared t -Se MTs, which are vital to study the photoelectric performance. The absorption of elemental selenium increases dramatically from nearly zero to a maximum value of ≈1.0 from 650 to 550 nm and then stays steady afterward. While the refl ection drops accordingly from ≈80% to ≈55% between 650 and 550 nm and then slowly decreases to ≈40% (350 nm). It is noteworthy that the Se-MTs exhibit both UV and visible light response with a cutoff wave- length estimated to be ≈660 nm.
Because the as fabricated Se-MTs are thick and long enough to be visible to the eyes, a single Se-MT is easily transferred to glass substrate and indium electrodes are then manually patterned on both sides of the microtube for device construc- tion as schematic illustration in Figure 3 a. The light active area is estimated to be 2.4 × 10 −8 m 2 . Incident light irradi- ates the device vertically. Figure 3 b shows the current–voltage ( I – V ) characteristics of the single Se-MT photodetector in dark, 350, 450, and 610 nm light illumination in semilogarithmic coordinates. I – V characterization in linear coordinates is also given in the inset of Figure 3 b. Linear I – V characte